Photoactivated surface grafting from PVDF surfaces Photoactivated surface grafting from PVDF...
Embed Size (px)
Transcript of Photoactivated surface grafting from PVDF surfaces Photoactivated surface grafting from PVDF...
Photoactivated surface grafting from PVDF surfaces
Thomas Berthelot, Xuan Tuan Le, Pascale Jégou, Pascal Viel, Bruno Boizot,
Cécile Baudin, Serge Palacin
To cite this version:
Thomas Berthelot, Xuan Tuan Le, Pascale Jégou, Pascal Viel, Bruno Boizot, et al.. Photoac- tivated surface grafting from PVDF surfaces. Applied Surface Science, Elsevier, 2011, 257, pp.9473. .
HAL Id: hal-00616622
Submitted on 23 Aug 2011
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Photoactivated surface grafting from PVDF surfaces
Thomas Berthelotb,∗, Xuan Tuan Leb, Pascale Jégoub, Pascal Vielb, Bruno Boizota,
Cécile Baudinb, Serge Palacinb a Laboratory of Irradiated Solids UMR 7642 CEA/CNRS/Ecole Polytechnique, CEA-DSM/IRAMIS LSI, Ecole
Polytechnique, F-91128, Palaiseau Cedex, France
b Chemistry of Surfaces and Interfaces, CEA Saclay, DSM/IRAMIS/SPCSI, F-91191, Gif-sur-Yvette Cedex, France
Economic and easy methods to tune surface properties of polymers as Poly(vinylidene fluoride)
(PVDF) without altering bulk properties are of major interest for different applications as
biotechnological devices, medical implant device... UV irradiation appears as one of the simplest,
easy and safe method to modify surface properties. In the case of self-initiated grafting, it is
generally assumed that the pretreatment of the PVDF surface with UV irradiation can yield alkyl
and peroxy radicals originating from breaking bonds and capable of initiating the subsequent
surface grafting polymerizations. Surprisingly, the present work shows that it is possible to obtain
polymer grafting using low energetic UV-A irradiation (3.1–3.9 eV) without breaking PVDF
bonds. An EPR study has been performed in order to investigate the nature of involved species.
The ability of the activated PVDF surface to graft different kinds of hydrophilic monomers using
the initiated surface polymerization method has been tested and discussed on the basis of ATR
FT-IR, XPS and NMR HRMAS result.
Poly(vinylidene fluoride) (PVDF) is a semi-crystalline and well known polymer which presents
excellent chemical and thermal stabilities and even compatibility with biological substances
including blood, food, etc. . The main disadvantage of PVDF is its non-reactivity towards
chemical compounds, which induces using complicated and expensive surface modifications
methods as plasma, irradiation (heavy ions, electrons, _-radiations), corona discharge, flame,
ozone treatment, ...  in order to improve its use for biotechnology as drug delivery system or
biosensors. It is thus interesting to find a simple and cheap surface modification method which
provides on one hand, fluoropolymer devices with different surface properties (hydrophilicity,
biocompatibility. . .) and on the other hand, keeps unaffected the bulk properties as flexibility,
piezoelectric or ferroelectric properties for example [2–4]. In the 1990s, the surface modification
of fluoropolymer films was shown to be induced by V-UV irradiation (100–200 nm) treatments
in oxidative or reductive atmospheres [5–7]. V-UV photons energy (6.2–12.4 eV) is sufficient to
break C F and/or C H bonds at the fluoropolymer surface resulting in radical production which
can eventually react with organic or gas molecules . More recent publications [8,9] proposed
various procedures for preparing polymer brushes from PVDF surfaces by UV-B irradiation (4.17
eV) and subsequent air exposure to create peroxide and hydroperoxide species which induce
direct surface polymerization. Surprisingly, we recently found that low-energy UV-A irradiation
(3.1–3.9 eV) can also induce polymer grafting by surface initiated polymerization, although its
energy is not enough to break CF or CH bonds. In order to investigate the actual nature of the
active species generated during UV-A irradiation of PVDF, we performed Electron Paramagnetic
Resonance (EPR) studies which are presented here. Reactivity of these UV-A-activated surfaces
towards different acrylate monomers is also reported and discussed on the basis of ATR FT-IR,
XPS and NMR HRMAS results.
Hydrophobic poly(vinylidene fluoride) films (PVDF , 9 µm thick, Solvay SA or Piezotech SA)
were Soxhlet extracted in toluene and dried at 50°C under vacuum. The PVDF films were sliced
into rectangular strips of size about 4 cm × 1.5 cm and then stored in nitrogen atmosphere. The
percentage of phase was obtained by the method described in  and was 67% for PVDF film
from Solvay SA and 64% for PVDF from Piezotech SA. Acrylic acid (Fluka) and 2-hydroxyethyl
methacrylate (Aldrich) were distilled under reduced pressure and stored in a nitrogen atmosphere
at 4°C before use. Water was MilliQ-grade. NaBH4, LiAlH4, acetonitrile and tetrahydrofuran
(THF) were purchased from Sigma–Aldrich and used as received.
2.2. UV-A irradiation
To overcome the high absorbance of Pyrex in the spectral range of UV-A, quartz tubes were used
during the irradiation step. After adding the PVDF film, the quartz tube was closed with silicon
rubber stopper and degassed with nitrogen for 30 min. The UV-A source was located at 4 cm
from the polymer film. The PVDF films were irradiated at room temperature for 15–60 min. The
UV-A light source (200 W) was a system (Omnicure Serie 2000) equipped with a high pressure
mercury lamp possessing an emission spectrum spanning the 320–500 nm range and a bandpass
filter. This UV system provides an irradiance level of 30 W cm−2 with maxima of light emission
at 369, 407 and 438 nm (Fig. 1). The collected light was analyzed by a SHAMROCK
spectrograph (F = 303 mm; 150 lines/mm grating and a 400 _m slit) combined with an ANDOR
Istar Intensified Charge-Coupled Device (ICCD).
2.3. Polymerization on the UV irradiated films
The exact conditions for the surface polymerization on the UV-irradiated PVDF films are
gathered in Table 1. Before the polymerization, the monomer and the solvent (if any) were de-
aerated separately by bubbling N2 gas for 1 h. They were then introduced into a degassed tube
containing the UV-A irradiated film for designated time (15–60 min). The sealed tube was put
into a thermo-stated bath at 60°C (see Table 1 for the duration). After polymerization, the film
was submitted to ultrasonic treatment in a good solvent of the corresponding monomer for 15
min. A Soxhlet extraction was then performed in water for 12 h and the resulting film was dried
under high vacuum. The polymerization and work-up conditions were summarized in Table 1.
2.4. Carbonyl reduction of PVDF surface
Surface PVDF films were submitted to two different protocols in order to reduce carbonyl group.
Protocol A: NaBH4 (100 mg, 2 mmol) were dissolved in 20 mL of MilliQ Water and then PVDF
films were disposed in this solution. After 3 h at 40°C, PVDF films were rinsed with 0.1 N HCl
solution and with ethanol. Resulting films were flushed with nitrogen gas and stocked under
Protocol B: 30 mL of THF were cooled at −30 ◦C with a liquid Nitrogen/Acetonitrile bath.
Afterwards, 100 mg of LiAlH4 (2.6 mmol) were added and PVDF films were disposed in the
resulting solution for 4 h. Finally, resulting PVDF films were rinsed with ethanol, flushed with
nitrogen gas and stocked under vacuum.
PVDF films obtained by these two protocols were analyzed by ATR FTIR and were submitted to
the same UV irradiation protocol and polymerization step described in the Sections 2.2 and 2.3.
2.5.1. EPR characterization
The EPR experiments were carried out at room temperature on a X band ( = 9.420 GHz) EMX
Bruker EPR spectrometer using a 100 kHz field modulation, 3 gauss (G) of amplitude modulation
and an applied microwave power of 1 mW. The spectra were obtained by sweeping the static
magnetic field (from 3275 to 3375 G) and by recording the first derivative of the absorption
spectrum. In order to compare the quantity of radical defects created by UV-A irradiation on
different experiments, all spectra were normalized to a sample weight of 100 mg and to a receiver
gain of 10 4 . A maximum error of 10% has been considered by taking into account the background
noise, the experimental errors on sample weight and on the sample position into the spectrometer